monoblocks in root canals
Post on 04-Nov-2014
Embed Size (px)
MONOBLOCKS IN ROOT CANALS: A FINITE ELEMENTAL STRESS ANALYSIS STUDY International Endodontic Journal 2011, VOL 44
GUIDED BY: DR B N KUMARASWAMY DR MANOJ KUMAR HANS DR SRIKUMAR DR KIRAN KESWANI PUNGA DR SUBHASH SINGH RAJPUTMANVA MOHNISH ZULFIKAR PRESENTED BY: PG STUDENT, DEPT. OF CONSERVATIVE DENTISTRY AND ENDODONTICS
The term monoblock, literally means a single unit.creating mechanically homogenous units with root dentin
Monoblock units can be created in a root canal system either by adhesive root canal sealers such as EndoREZ, RealSeal, Epiphany or MetaSEAL in combination with a bondable root
Monoblocks can also be created using adhesive post systems, which have similar elastic moduli to dentine such as carbon fibrereinforced posts, prefabricated glass-fibre posts, customized polyethylene fibre posts or customized glass-fibre posts.
Tay & Pashley 2007
OBTURATION MTA, NEC, CEM
POST & CORE COSTOMIZED POLYTHYLENE FIBRE POST-CORE SYSTEM CAST POST, PREFEB METAL
CONVENTIONAL, RESILONEPIPHENY/ENDOREZ/ REALSEAL/MEATASEA L GP+BONDING +RESIN SEALER
FIBRE POST, GLASS FIB,CERAMIC POST
to evaluate the effect of different monoblock models on stress distribution in remaining tooth structures.The hypothesis tested was that increased interfaces created in FEA monoblock models either by an endodontic or by post-core material do not have an effect on stress distribution.
MATERIAL & METHODS7
A 3-D FEA method and a FE structural analysis programme. Three-dimensional maxillary central incisor FEA models were created including the following structures: enamel(e); dentine(d); composite resin(c); guttapercha(g); ceramic restoration(cr), resin-core(rc); post(p)
The models were modified to demonstrate(i)primary monoblock with MTA; (ii) secondary monoblock with MetaSEAL and Resilon; (iii) tertiary monoblock with EndoREZ; (iv) primary monoblock with polyethylene fibre postcore system; (v) secondary monoblock with glass-fibre post and resin cement; (vi) tertiary monoblock with bondable glass-fibre post; (vii) tertiary monoblock with silane-coated ceramic
Materials used in the study were assumed as homogenous and isotropic except the glass-fibre post.
The glass-fibre post was considered to be made of long fibres (glass-fibre) embedded into a polymeric matrix.Considered orthotropic, so that it shows different mechanical properties along the fibre direction and along the other two normal
ELASTIC PROPERTIES OF ISOTROPIC MATERIALS11
RESIN CORECERAMIC VENEER POLYETHYLENE FIBRE COMPOSITE DENTINE
9565 23.6 12 18.6
0.240.24 0.32 0.30 0.31
RESIN CEMENTGUTTA PERCHA RESILON ADHESIVE MTA
80.076 0.107 10.5 22.5
0.300.45 0.45 0.28 0.314
ELASTIC PROPERTIES OF ORTHOTROPIC MATERIALS12
PROPERTY EX EY EZ NUXY NUXZ NUYZ GXY GXZ GYZ
GLASS POST 37 9.5 9.5 0.27 0.34 0.27 3.10 3.50 3.10
Ex, Ey and Ez represent the elastic moduli along the three directions, whilst NUxy, NUxz, NUyz and Gxy, Gxz, Gyz are, respectively, the Poissons ratios and the shear moduli in the orthogonal planes
An occlusal force of 300 N was applied from the palatal surface of the crown at a 135 angle to the tooth long axis.Nodes at the outer surface of roots were assumed as fixed in all directions to calculate the stress distribution
Calculated numeric data were transformed into colour graphics to better visualize mechanical phenomena in the models.The FEA results are presented as stresses distributed in the investigated structures. Results are presented by considering von Mises criteria.
The palatal side of the MTA model showed a decreased stress accumulation (8.3313.3 MPa) when compared to the others.
It is obvious that the composite resin in the access cavity has changed the stress direction when compared to the natural tooth structure and increased stress at the coronal region
The MTA-treated model revealed that the material kept the stress inside of the material body (1.67-3.33 MPa) and directed towards the root via the root canal; therefore, stress at the palatal cervical region decreased under loading
On the other hand, the secondary monoblock model revealed stress accumulation at the interface between the Resilon and MetaSEAL
Stress distribution through the guttapercha (5 6.67 MPa) increased in the tertiary monoblock model created by EndoREZ.
In contrast to the other endodontic models (1.673.33 MPa), the stress values at the interface were high in this model (6.6710 MPa).
The primary monoblock model created with polyethylene fibre revealed stress distribution at the coronal region ranging from 1.57 to 5 MPa but not in the root structure when compared to the tertiary monoblock models, which were created either by bondable glassfibre posts (6.6710 MPa) or by silanecoated ceramic posts (6.6713.3 MPa).
Primary (polyethylene fibre post) and secondary monoblock (glass-fibre post) models showed similar stress values and distribution at the coronal region decreasing towards the root (from 6.67 to 1.67 MPa).
Stress values along the cement glassfibre or ceramic interface ranged from 1.67 to 15 Mpa for tertiary monoblock models (bondable glass-fibre; 1.675 MPa and the silane-coated ceramic post; 1.67 15 MPa).
Furthermore, the stress was directed through the root in tertiary monoblock models. In contrast to the glass-fibre post, the ceramic post retained the stress inside the body of the post.
This study was built on the assumption that a monoblock can be achieved in root canal treatment and the placement of post-core.The concept of creating mechanically homogenous units within root dentine is excellent in theory; however, accomplishing these ideal monoblocks in the canal space is challenging.
Accuracy of the experimental model is crucial for the validity of the results of a FEA study. FEA consists of a computer model of a material or design that is stressed and analysed for specific results.
The first issue to understand in FEA is that it is fundamentally an approximation
On the other hand, FEA analysis, models and simulations have been used for many years to estimate the biomechanical behaviour of materials and structures where these predicted variables are impossible to measure directly (Eskitascioglu et al. 2002, Apicella 2008).
Furthermore, previous studies indicated that FEM results confirm the results of laboratory studies (Eskitascioglu et al. 2002, Asmussen et al. 2005).
Several techniques and methods can be used to evaluate distribution of functional stresses in a structure including photoelastic studies, 2dimensional FEA or 3-dimensional FEA (Dietschi et al. 2007). Threedimensional FEA is generally preferred to obtain a realistic analysis because 2dimensional modelling may not represent tooth irregularities and may neglect several important details
In the present study, a 3-dimensional FEA method was used to evaluate the pattern of stress distribution in the roots filled either with endodontic materials or restored with different post-core systems. The FEA model used was based on a maxillary incisor.
Three-dimensional models were constructed for this purpose, and the structures in the models were all assumed to be homogeneous isotropic and possess linear elasticity except the glassfibre post.
The majority of the fibre-reinforced composite (FRC) posts contain a resin matrix with embedded glass or quartz fibres.
The fibres are designed to provide high tensile strength, and the resin matrix is supposed to withstand compressive stresses and absorb stresses in the entire post system
The mechanical behaviours of fibre-reinforced posts depend on many factors such as direction or orientation of the fibres, individual properties of fibres and matrix, the density, diameter and adhesion of the fibres to the resin matrix, etc.
The FEM results are presented as stresses distributed in the investigated structures. These stresses may occur as tensile, compressive, shear or a stress combination. The global (x, y and z directional axes) combination of the absolute values squared of all stresses is known as von Mises stresses (RicksWilliamson et al. 1995). Von Mises stresses depend on the entire stress field and are widely used as an indicator of the
Contrary to the normal tooth, more stress concentrated in the remaining tooth structure especially in the tertiary monoblock created models (Figs 4 and 5). The stress inside the root structure increased with the increased interfaces.
This result confirms the concept that the interfaces of materials with different moduli of elasticity represent the weak point of a restorative system, as the toughness/stiffness mismatch influences the stress distribution
The major changes in tooth biomechanics are attributed to the loss of tissue in root filled teeth. In a biomechanical aspect, restoration of root filled teeth with materials having a similar elastic modulus to dentine can save the remaining tooth structure. In other words, rigid materials can lead to failure of the restorations or can result in fracture of the remaining tooth structure.
Metals and ceramics used for post fabrication p